#------------------------------------------------------------------------------
#$Date: 2025-07-01 14:32:45 +0300 (Tue, 01 Jul 2025) $
#$Revision: 1289 $
#$URL: svn://crystallography.net/testcod/cif/4/00/00/4000073.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4000073
loop_
_publ_author_name
'Porras-Vázquez, José M.'
'Losilla, Enrique R.'
'León-Reina, Laura'
'Martínez-Lara, María'
'Aranda, Miguel A. G.'
_publ_section_title
;
 Synthesis and Characterization of a New Family of Mixed
 Oxide−Proton Conductors Based on Tristrontium Oxysilicate
;
_journal_issue                   5
_journal_name_full               'Chemistry of Materials'
_journal_page_first              2026
_journal_page_last               2034
_journal_paper_doi               10.1021/cm703079d
_journal_volume                  20
_journal_year                    2008
_chemical_formula_sum            'O5 Si Sr3'
_chemical_formula_weight         370.94
_space_group_IT_number           130
_space_group_name_Hall           '-P 4a 2ac'
_space_group_name_H-M_alt        'P 4/n c c :2'
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_H-M   'P 4/n c c :2'
_audit_creation_date             2007-09-13T18:31
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
' 2007-09-13T18:31  Initial CIF as created by GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            4
_cell_length_a                   6.951343(33)
_cell_length_b                   6.951343
_cell_length_c                   10.76111(6)
_cell_volume                     519.989(4)
_computing_structure_refinement  GSAS
_pd_block_id                     2007-09-13T18:31|Sr3SiO5|Aranda_MAG|Sr3SiO5
_pd_phase_name
'from C:/Rietveld/Jose_Manuel/Serie_SrSi(Al)/Sr3SiO5/Sintesis_2/SR3'
_refine_ls_goodness_of_fit_all   2.27
_refine_ls_matrix_type           full
_refine_ls_number_parameters     52
_refine_ls_number_restraints     0
_refine_ls_shift/su_max          0.08
_refine_ls_shift/su_mean         0.01
_cod_data_source_file            cm703079d-file001.cif
_cod_data_source_block           Sr3SiO5_publ
_cod_original_cell_volume        519.990(7)
_cod_original_sg_symbol_H-M      'P 4/n c c'
_cod_database_code               4000073
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 -y+1/2,+x,+z
3 -x+1/2,-y+1/2,+z
4 +y,-x+1/2,+z
5 -x+1/2,+y,+z+1/2
6 -y+1/2,-x+1/2,+z+1/2
7 +x,-y+1/2,+z+1/2
8 +y,+x,+z+1/2
-1 -x,-y,-z
-2 +y+1/2,-x,-z
-3 +x+1/2,+y+1/2,-z
-4 -y,+x+1/2,-z
-5 +x+1/2,-y,-z+1/2
-6 +y+1/2,+x+1/2,-z+1/2
-7 -x,+y+1/2,-z+1/2
-8 -y,-x,-z+1/2
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
Sr Sr1 0.43755(7) 0.93755(7) 0.75 1.0 Uiso 0.00552 8
Sr Sr2 0.25 0.25 -0.00855(13) 1.0 Uiso 0.00882 4
Si Si1 0.25 0.75 0.0 1.0 Uiso 0.00098 4
O O1 0.4053(5) 0.6454(5) 0.59112(27) 1.0 Uiso 0.00663 16
O O2 0.25 0.25 0.2248(6) 1.0 Uiso 0.0019 4
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Sr1 Sr1 Sr1 151.950(29) 2_655 . 2_665 N
Sr1 Sr1 Sr1 59.025(14) 2_655 . 3_565 N
Sr1 Sr1 Sr1 118.050(29) 2_655 . 4_465 N
Sr1 Sr1 Sr1 90.0 2_655 . 4_565 N
Sr1 Sr1 Sr2 131.894(17) 2_655 . 1_566 N
Sr1 Sr1 Sr2 130.090(16) 2_655 . 5_565 N
Sr1 Sr1 Sr2 61.572(9) 2_655 . -1_666 N
Sr1 Sr1 Sr2 60.422(9) 2_655 . -5_556 N
Sr1 Sr1 Si1 73.085(12) 2_655 . 1_556 N
Sr1 Sr1 Si1 73.085(12) 2_655 . 5_555 N
Sr1 Sr1 O1 44.02(7) 2_655 . 1_555 N
Sr1 Sr1 O1 90.35(7) 2_655 . 3_565 N
Sr1 Sr1 O1 106.56(9) 2_655 . 4_565 N
Sr1 Sr1 O1 95.91(8) 2_655 . -6_466 N
Sr1 Sr1 O1 117.16(9) 2_655 . -7_566 N
Sr1 Sr1 O1 43.39(6) 2_655 . -8_566 N
Sr1 Sr1 O2 162.01(6) 2_655 . 5_565 N
Sr1 Sr1 O2 45.325(16) 2_655 . -1_666 N
Sr1 Sr1 Sr1 149.025(14) 2_665 . 3_565 N
Sr1 Sr1 Sr1 90.0 2_665 . 4_465 N
Sr1 Sr1 Sr1 61.950(29) 2_665 . 4_565 N
Sr1 Sr1 Sr2 60.421(9) 2_665 . 1_566 N
Sr1 Sr1 Sr2 61.572(9) 2_665 . 5_565 N
Sr1 Sr1 Sr2 101.319(19) 2_665 . -1_666 N
Sr1 Sr1 Sr2 101.743(20) 2_665 . -5_556 N
Sr1 Sr1 Si1 118.9928(29) 2_665 . 1_556 N
Sr1 Sr1 Si1 118.9928(29) 2_665 . 5_555 N
Sr1 Sr1 O1 139.46(7) 2_665 . 1_555 N
Sr1 Sr1 O1 112.36(7) 2_665 . 3_565 N
Sr1 Sr1 O1 55.52(8) 2_665 . 4_565 N
Sr1 Sr1 O1 105.46(8) 2_665 . -6_466 N
Sr1 Sr1 O1 48.01(8) 2_665 . -7_566 N
Sr1 Sr1 O1 145.11(6) 2_665 . -8_566 N
Sr1 Sr1 O2 45.325(16) 2_665 . 5_565 N
Sr1 Sr1 O2 106.851(29) 2_665 . -1_666 N
Sr1 Sr1 Sr1 59.025(14) 3_565 . 4_465 N
Sr1 Sr1 Sr1 149.025(14) 3_565 . 4_565 N
Sr1 Sr1 Sr2 99.740(10) 3_565 . 1_566 N
Sr1 Sr1 Sr2 99.390(10) 3_565 . 5_565 N
Sr1 Sr1 Sr2 99.390(10) 3_565 . -1_666 N
Sr1 Sr1 Sr2 99.740(10) 3_565 . -5_556 N
Sr1 Sr1 Si1 55.575(9) 3_565 . 1_556 N
Sr1 Sr1 Si1 55.575(9) 3_565 . 5_555 N
Sr1 Sr1 O1 53.23(8) 3_565 . 1_555 N
Sr1 Sr1 O1 45.56(7) 3_565 . 3_565 N
Sr1 Sr1 O1 136.08(7) 3_565 . 4_565 N
Sr1 Sr1 O1 53.23(8) 3_565 . -6_466 N
Sr1 Sr1 O1 136.08(7) 3_565 . -7_566 N
Sr1 Sr1 O1 45.56(7) 3_565 . -8_566 N
Sr1 Sr1 O2 103.943(15) 3_565 . 5_565 N
Sr1 Sr1 O2 103.944(15) 3_565 . -1_666 N
Sr1 Sr1 Sr1 151.950(29) 4_465 . 4_565 N
Sr1 Sr1 Sr2 60.421(9) 4_465 . 1_566 N
Sr1 Sr1 Sr2 61.572(9) 4_465 . 5_565 N
Sr1 Sr1 Sr2 130.090(16) 4_465 . -1_666 N
Sr1 Sr1 Sr2 131.894(17) 4_465 . -5_556 N
Sr1 Sr1 Si1 73.085(12) 4_465 . 1_556 N
Sr1 Sr1 Si1 73.085(12) 4_465 . 5_555 N
Sr1 Sr1 O1 95.91(8) 4_465 . 1_555 N
Sr1 Sr1 O1 43.39(6) 4_465 . 3_565 N
Sr1 Sr1 O1 117.16(9) 4_465 . 4_565 N
Sr1 Sr1 O1 44.02(7) 4_465 . -6_466 N
Sr1 Sr1 O1 106.56(9) 4_465 . -7_566 N
Sr1 Sr1 O1 90.35(7) 4_465 . -8_566 N
Sr1 Sr1 O2 45.325(16) 4_465 . 5_565 N
Sr1 Sr1 O2 162.01(6) 4_465 . -1_666 N
Sr1 Sr1 Sr2 101.743(20) 4_565 . 1_566 N
Sr1 Sr1 Sr2 101.319(19) 4_565 . 5_565 N
Sr1 Sr1 Sr2 61.572(9) 4_565 . -1_666 N
Sr1 Sr1 Sr2 60.422(9) 4_565 . -5_556 N
Sr1 Sr1 Si1 118.9930(29) 4_565 . 1_556 N
Sr1 Sr1 Si1 118.9930(29) 4_565 . 5_555 N
Sr1 Sr1 O1 105.46(8) 4_565 . 1_555 N
Sr1 Sr1 O1 145.11(6) 4_565 . 3_565 N
Sr1 Sr1 O1 48.01(8) 4_565 . 4_565 N
Sr1 Sr1 O1 139.46(7) 4_565 . -6_466 N
Sr1 Sr1 O1 55.52(8) 4_565 . -7_566 N
Sr1 Sr1 O1 112.36(7) 4_565 . -8_566 N
Sr1 Sr1 O2 106.851(29) 4_565 . 5_565 N
Sr1 Sr1 O2 45.325(16) 4_565 . -1_666 N
Sr2 Sr1 Sr2 93.410(4) 1_566 . 5_565 N
Sr2 Sr1 Sr2 83.4148(32) 1_566 . -1_666 N
Sr2 Sr1 Sr2 160.520(21) 1_566 . -5_556 N
Sr2 Sr1 Si1 60.331(13) 1_566 . 1_556 N
Sr2 Sr1 Si1 133.335(14) 1_566 . 5_555 N
Sr2 Sr1 O1 152.31(8) 1_566 . 1_555 N
Sr2 Sr1 O1 103.80(6) 1_566 . 3_565 N
Sr2 Sr1 O1 115.93(9) 1_566 . 4_565 N
Sr2 Sr1 O1 46.93(8) 1_566 . -6_466 N
Sr2 Sr1 O1 47.08(9) 1_566 . -7_566 N
Sr2 Sr1 O1 89.90(6) 1_566 . -8_566 N
Sr2 Sr1 O2 51.84(16) 1_566 . 5_565 N
Sr2 Sr1 O2 122.43(15) 1_566 . -1_666 N
Sr2 Sr1 Sr2 161.220(21) 5_565 . -1_666 N
Sr2 Sr1 Sr2 83.4148(32) 5_565 . -5_556 N
Sr2 Sr1 Si1 134.601(14) 5_565 . 1_556 N
Sr2 Sr1 Si1 58.822(12) 5_565 . 5_555 N
Sr2 Sr1 O1 86.35(7) 5_565 . 1_555 N
Sr2 Sr1 O1 54.00(7) 5_565 . 3_565 N
Sr2 Sr1 O1 55.96(9) 5_565 . 4_565 N
Sr2 Sr1 O1 105.01(7) 5_565 . -6_466 N
Sr2 Sr1 O1 108.95(8) 5_565 . -7_566 N
Sr2 Sr1 O1 144.72(7) 5_565 . -8_566 N
Sr2 Sr1 O2 41.57(16) 5_565 . 5_565 N
Sr2 Sr1 O2 132.03(14) 5_565 . -1_666 N
Sr2 Sr1 Sr2 93.410(4) -1_666 . -5_556 N
Sr2 Sr1 Si1 58.822(12) -1_666 . 1_556 N
Sr2 Sr1 Si1 134.601(14) -1_666 . 5_555 N
Sr2 Sr1 O1 105.01(7) -1_666 . 1_555 N
Sr2 Sr1 O1 144.72(7) -1_666 . 3_565 N
Sr2 Sr1 O1 108.95(8) -1_666 . 4_565 N
Sr2 Sr1 O1 86.35(7) -1_666 . -6_466 N
Sr2 Sr1 O1 55.96(9) -1_666 . -7_566 N
Sr2 Sr1 O1 54.00(7) -1_666 . -8_566 N
Sr2 Sr1 O2 132.03(14) -1_666 . 5_565 N
Sr2 Sr1 O2 41.57(16) -1_666 . -1_666 N
Sr2 Sr1 Si1 133.335(14) -5_656 . 1_556 N
Sr2 Sr1 Si1 60.331(13) -5_656 . 5_555 N
Sr2 Sr1 O1 46.93(8) -5_565 . 1_555 N
Sr2 Sr1 O1 89.90(6) -5_565 . 3_565 N
Sr2 Sr1 O1 47.08(9) -5_565 . 4_565 N
Sr2 Sr1 O1 152.31(8) -5_565 . -6_466 N
Sr2 Sr1 O1 115.93(9) -5_565 . -7_566 N
Sr2 Sr1 O1 103.80(6) -5_565 . -8_566 N
Sr2 Sr1 O2 122.43(15) -5_555 . 5_565 N
Sr2 Sr1 O2 51.84(16) -5_555 . -1_666 N
Si1 Sr1 Si1 111.151(19) 1_556 . 5_555 N
Si1 Sr1 O1 101.01(7) 1_556 . 1_555 N
Si1 Sr1 O1 94.36(7) 1_556 . 3_565 N
Si1 Sr1 O1 166.76(8) 1_556 . 4_565 N
Si1 Sr1 O1 29.80(7) 1_556 . -6_466 N
Si1 Sr1 O1 80.85(7) 1_556 . -7_566 N
Si1 Sr1 O1 29.82(6) 1_556 . -8_566 N
Si1 Sr1 O2 102.95(13) 1_556 . 5_565 N
Si1 Sr1 O2 92.77(13) 1_556 . -1_666 N
Si1 Sr1 O1 29.80(7) 5_555 . 1_555 N
Si1 Sr1 O1 29.82(6) 5_555 . 3_565 N
Si1 Sr1 O1 80.85(7) 5_555 . 4_565 N
Si1 Sr1 O1 101.01(7) 5_555 . -6_466 N
Si1 Sr1 O1 166.76(8) 5_555 . -7_566 N
Si1 Sr1 O1 94.36(7) 5_555 . -8_566 N
Si1 Sr1 O2 92.77(13) 5_555 . 5_565 N
Si1 Sr1 O2 102.95(13) 5_555 . -1_666 N
O1 Sr1 O1 54.46(13) 1_555 . 3_565 N
O1 Sr1 O1 86.72(14) 1_555 . 4_565 N
O1 Sr1 O1 106.46(15) 1_555 . -6_466 N
O1 Sr1 O1 156.87(7) 1_555 . -7_566 N
O1 Sr1 O1 75.11(10) 1_555 . -8_566 N
O1 Sr1 O2 122.57(15) 1_555 . 5_565 N
O1 Sr1 O2 75.53(13) 1_555 . -1_666 N
O1 Sr1 O1 98.88(13) 3_565 . 4_565 N
O1 Sr1 O1 75.11(10) 3_565 . -6_466 N
O1 Sr1 O1 148.68(11) 3_565 . -7_566 N
O1 Sr1 O1 91.12(13) 3_565 . -8_566 N
O1 Sr1 O2 72.28(11) 3_565 . 5_565 N
O1 Sr1 O2 129.93(12) 3_565 . -1_666 N
O1 Sr1 O1 156.87(7) 4_565 . -6_466 N
O1 Sr1 O1 87.83(15) 4_565 . -7_566 N
O1 Sr1 O1 148.68(11) 4_565 . -8_566 N
O1 Sr1 O2 81.36(13) 4_565 . 5_565 N
O1 Sr1 O2 78.64(13) 4_565 . -1_666 N
O1 Sr1 O1 86.72(14) -6_466 . -7_566 N
O1 Sr1 O1 54.46(13) -6_466 . -8_566 N
O1 Sr1 O2 75.53(13) -6_456 . 5_565 N
O1 Sr1 O2 122.57(15) -6_456 . -1_666 N
O1 Sr1 O1 98.88(13) -7_566 . -8_566 N
O1 Sr1 O2 78.64(13) -7_556 . 5_565 N
O1 Sr1 O2 81.36(13) -7_556 . -1_666 N
O1 Sr1 O2 129.93(12) -8_556 . 5_565 N
O1 Sr1 O2 72.28(11) -8_556 . -1_666 N
O2 Sr1 O2 152.113(30) 5_565 . -1_666 N
Sr1 Sr2 Sr1 59.157(19) 1_544 . 2_654 N
Sr1 Sr2 Sr1 88.546(32) 1_544 . 3_564 N
Sr1 Sr2 Sr1 59.157(19) 1_544 . 4_454 N
Sr1 Sr2 Sr1 107.966(15) 1_544 . 5_544 N
Sr1 Sr2 Sr1 96.5851(32) 1_544 . 6_654 N
Sr1 Sr2 Sr1 138.629(17) 1_544 . 7_564 N
Sr1 Sr2 Sr1 160.772(20) 1_544 . 8_454 N
Sr1 Sr2 O1 104.38(8) 1_544 . -5_465 N
Sr1 Sr2 O1 47.09(8) 1_544 . -6_455 N
Sr1 Sr2 O1 43.35(7) 1_544 . -7_555 N
Sr1 Sr2 O1 101.66(8) 1_544 . -8_565 N
Sr1 Sr2 O2 135.727(16) 1_544 . 1_555 N
Sr1 Sr2 O2 44.273(16) 1_544 . 5_554 N
Sr1 Sr2 Sr1 59.157(19) 2_654 . 3_564 N
Sr1 Sr2 Sr1 88.546(32) 2_654 . 4_454 N
Sr1 Sr2 Sr1 160.772(20) 2_654 . 5_544 N
Sr1 Sr2 Sr1 107.966(15) 2_654 . 6_654 N
Sr1 Sr2 Sr1 96.5851(32) 2_654 . 7_564 N
Sr1 Sr2 Sr1 138.629(17) 2_654 . 8_454 N
Sr1 Sr2 O1 101.66(8) 2_654 . -5_465 N
Sr1 Sr2 O1 104.38(8) 2_654 . -6_455 N
Sr1 Sr2 O1 47.09(8) 2_654 . -7_555 N
Sr1 Sr2 O1 43.35(7) 2_654 . -8_565 N
Sr1 Sr2 O2 135.727(16) 2_654 . 1_555 N
Sr1 Sr2 O2 44.273(16) 2_654 . 5_554 N
Sr1 Sr2 Sr1 59.157(19) 3_564 . 4_454 N
Sr1 Sr2 Sr1 138.629(17) 3_564 . 5_544 N
Sr1 Sr2 Sr1 160.772(20) 3_564 . 6_654 N
Sr1 Sr2 Sr1 107.966(15) 3_564 . 7_564 N
Sr1 Sr2 Sr1 96.5851(32) 3_564 . 8_454 N
Sr1 Sr2 O1 43.35(7) 3_564 . -5_465 N
Sr1 Sr2 O1 101.66(8) 3_564 . -6_455 N
Sr1 Sr2 O1 104.38(8) 3_564 . -7_555 N
Sr1 Sr2 O1 47.09(8) 3_564 . -8_565 N
Sr1 Sr2 O2 135.727(16) 3_564 . 1_555 N
Sr1 Sr2 O2 44.273(16) 3_564 . 5_554 N
Sr1 Sr2 Sr1 96.5851(32) 4_454 . 5_544 N
Sr1 Sr2 Sr1 138.629(17) 4_454 . 6_654 N
Sr1 Sr2 Sr1 160.772(20) 4_454 . 7_564 N
Sr1 Sr2 Sr1 107.966(15) 4_454 . 8_454 N
Sr1 Sr2 O1 47.09(8) 4_454 . -5_465 N
Sr1 Sr2 O1 43.35(7) 4_454 . -6_455 N
Sr1 Sr2 O1 101.66(8) 4_454 . -7_555 N
Sr1 Sr2 O1 104.38(8) 4_454 . -8_565 N
Sr1 Sr2 O2 135.727(16) 4_454 . 1_555 N
Sr1 Sr2 O2 44.273(16) 4_454 . 5_554 N
Sr1 Sr2 Sr1 56.855(18) 5_544 . 6_654 N
Sr1 Sr2 Sr1 84.634(30) 5_544 . 7_564 N
Sr1 Sr2 Sr1 56.855(18) 5_544 . 8_454 N
Sr1 Sr2 O1 95.32(7) 5_544 . -5_465 N
Sr1 Sr2 O1 68.40(7) 5_544 . -6_455 N
Sr1 Sr2 O1 113.69(8) 5_544 . -7_555 N
Sr1 Sr2 O1 149.61(8) 5_544 . -8_565 N
Sr1 Sr2 O2 42.317(15) 5_544 . 1_555 N
Sr1 Sr2 O2 137.683(15) 5_544 . 5_554 N
Sr1 Sr2 Sr1 56.855(18) 6_654 . 7_564 N
Sr1 Sr2 Sr1 84.634(30) 6_654 . 8_454 N
Sr1 Sr2 O1 149.61(8) 6_654 . -5_465 N
Sr1 Sr2 O1 95.32(7) 6_654 . -6_455 N
Sr1 Sr2 O1 68.40(7) 6_654 . -7_555 N
Sr1 Sr2 O1 113.69(8) 6_654 . -8_565 N
Sr1 Sr2 O2 42.317(15) 6_654 . 1_555 N
Sr1 Sr2 O2 137.683(15) 6_654 . 5_554 N
Sr1 Sr2 Sr1 56.855(18) 7_564 . 8_454 N
Sr1 Sr2 O1 113.69(8) 7_564 . -5_465 N
Sr1 Sr2 O1 149.61(8) 7_564 . -6_455 N
Sr1 Sr2 O1 95.32(7) 7_564 . -7_555 N
Sr1 Sr2 O1 68.40(7) 7_564 . -8_565 N
Sr1 Sr2 O2 42.317(15) 7_564 . 1_555 N
Sr1 Sr2 O2 137.683(15) 7_564 . 5_554 N
Sr1 Sr2 O1 68.40(7) 8_454 . -5_465 N
Sr1 Sr2 O1 113.69(8) 8_454 . -6_455 N
Sr1 Sr2 O1 149.61(8) 8_454 . -7_555 N
Sr1 Sr2 O1 95.32(7) 8_454 . -8_565 N
Sr1 Sr2 O2 42.317(15) 8_454 . 1_555 N
Sr1 Sr2 O2 137.683(15) 8_454 . 5_554 N
O1 Sr2 O1 83.58(5) -5_465 . -6_455 N
O1 Sr2 O1 140.93(15) -5_465 . -7_555 N
O1 Sr2 O1 83.58(5) -5_465 . -8_565 N
O1 Sr2 O2 109.54(8) -5_455 . 1_555 N
O1 Sr2 O2 70.46(8) -5_455 . 5_554 N
O1 Sr2 O1 83.58(5) -6_455 . -7_555 N
O1 Sr2 O1 140.93(15) -6_455 . -8_565 N
O1 Sr2 O2 109.54(8) -6_445 . 1_555 N
O1 Sr2 O2 70.46(8) -6_445 . 5_554 N
O1 Sr2 O1 83.58(5) -7_555 . -8_565 N
O1 Sr2 O2 109.54(8) -7_545 . 1_555 N
O1 Sr2 O2 70.46(8) -7_545 . 5_554 N
O1 Sr2 O2 109.54(8) -8_555 . 1_555 N
O1 Sr2 O2 70.46(8) -8_555 . 5_554 N
O2 Sr2 O2 180.0 1_555 . 5_554 N
Sr1 Si1 Sr1 68.849(19) 1_554 . 3_564 N
Sr1 Si1 Sr1 132.876(12) 1_554 . 5_554 N
Sr1 Si1 Sr1 132.876(12) 1_554 . 7_564 N
Sr1 Si1 O1 159.98(11) 1_554 . 5_554 N
Sr1 Si1 O1 93.05(11) 1_554 . 7_564 N
Sr1 Si1 O1 54.35(12) 1_554 . -6_465 N
Sr1 Si1 O1 65.79(12) 1_554 . -8_565 N
Sr1 Si1 Sr1 132.876(12) 3_564 . 5_554 N
Sr1 Si1 Sr1 132.876(12) 3_564 . 7_564 N
Sr1 Si1 O1 93.05(11) 3_564 . 5_554 N
Sr1 Si1 O1 159.98(11) 3_564 . 7_564 N
Sr1 Si1 O1 65.79(12) 3_564 . -6_465 N
Sr1 Si1 O1 54.35(12) 3_564 . -8_565 N
Sr1 Si1 Sr1 68.849(19) 5_554 . 7_564 N
Sr1 Si1 O1 54.35(12) 5_554 . 5_554 N
Sr1 Si1 O1 65.79(12) 5_554 . 7_564 N
Sr1 Si1 O1 93.05(11) 5_554 . -6_465 N
Sr1 Si1 O1 159.98(11) 5_554 . -8_565 N
Sr1 Si1 O1 65.79(12) 7_564 . 5_554 N
Sr1 Si1 O1 54.35(12) 7_564 . 7_564 N
Sr1 Si1 O1 159.98(11) 7_564 . -6_465 N
Sr1 Si1 O1 93.05(11) 7_564 . -8_565 N
O1 Si1 O1 106.00(22) 5_554 . 7_564 N
O1 Si1 O1 111.23(11) 5_554 . -6_465 N
O1 Si1 O1 111.23(11) 5_554 . -8_565 N
O1 Si1 O1 111.23(11) 7_564 . -6_465 N
O1 Si1 O1 111.23(11) 7_564 . -8_565 N
O1 Si1 O1 106.00(22) -6_465 . -8_565 N
Sr1 O1 Sr1 87.98(10) 1_555 . 2_655 N
Sr1 O1 Sr1 81.21(8) 1_555 . 3_565 N
Sr1 O1 Sr2 85.99(12) 1_555 . -5_556 N
Sr1 O1 Si1 95.84(15) 1_555 . 5_555 N
Sr1 O1 Sr1 81.10(9) 2_655 . 3_565 N
Sr1 O1 Sr2 89.58(12) 2_655 . -5_556 N
Sr1 O1 Si1 164.25(21) 2_655 . 5_555 N
Sr1 O1 Sr2 164.37(14) 3_565 . -5_556 N
Sr1 O1 Si1 84.39(14) 3_565 . 5_555 N
Sr2 O1 Si1 105.90(15) -5_656 . 5_555 N
Sr1 O2 Sr1 89.350(33) 5_544 . 6_654 N
Sr1 O2 Sr1 167.77(31) 5_544 . 7_564 N
Sr1 O2 Sr1 89.350(33) 5_544 . 8_454 N
Sr1 O2 Sr2 96.11(16) 5_544 . 1_555 N
Sr1 O2 Sr2 83.89(16) 5_544 . 5_555 N
Sr1 O2 Sr1 89.350(33) 6_654 . 7_564 N
Sr1 O2 Sr1 167.77(31) 6_654 . 8_454 N
Sr1 O2 Sr2 96.11(16) 6_654 . 1_555 N
Sr1 O2 Sr2 83.89(16) 6_654 . 5_555 N
Sr1 O2 Sr1 89.350(33) 7_564 . 8_454 N
Sr1 O2 Sr2 96.11(16) 7_564 . 1_555 N
Sr1 O2 Sr2 83.89(16) 7_564 . 5_555 N
Sr1 O2 Sr2 96.11(16) 8_454 . 1_555 N
Sr1 O2 Sr2 83.89(16) 8_454 . 5_555 N
Sr2 O2 Sr2 179.9657 1_555 . 5_555 N
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Sr1 Sr1 3.58246(22) . 2_655 N
Sr1 Sr1 3.58247(22) . 2_665 N
Sr1 Sr1 3.6875(13) . 3_565 N
Sr1 Sr1 3.58247(22) . 4_465 N
Sr1 Sr1 3.58246(22) . 4_565 N
Sr1 Sr2 3.6288(10) . 1_566 N
Sr1 Sr2 3.7627(11) . 5_565 N
Sr1 Sr2 3.7627(11) . -1_666 N
Sr1 Sr2 3.6288(10) . -5_565 N
Sr1 Si1 3.2615(4) . 1_556 N
Sr1 Si1 3.2615(4) . 5_555 N
Sr1 O1 2.6642(34) . 1_555 N
Sr1 O1 2.989(4) . 3_565 N
Sr1 O1 2.4909(32) . 4_565 N
Sr1 O1 2.6642(34) . -6_456 N
Sr1 O1 2.4909(32) . -7_656 N
Sr1 O1 2.989(4) . -8_666 N
Sr1 O2 2.5477(8) . 5_565 N
Sr1 O2 2.5477(8) . -1_666 N
Sr2 Sr1 3.6288(10) . 1_544 N
Sr2 Sr1 3.6288(10) . 2_654 N
Sr2 Sr1 3.6288(10) . 3_564 N
Sr2 Sr1 3.6288(10) . 4_454 N
Sr2 Sr1 3.7627(11) . 5_544 N
Sr2 Sr1 3.7627(11) . 6_654 N
Sr2 Sr1 3.7627(11) . 7_564 N
Sr2 Sr1 3.7627(11) . 8_454 N
Sr2 Si1 3.47689(4) . 1_545 N
Sr2 Si1 3.47689(4) . 1_555 N
Sr2 Si1 3.47689(4) . 2_555 N
Sr2 Si1 3.47689(4) . 2_655 N
Sr2 O1 3.142(4) . 5_554 N
Sr2 O1 3.142(4) . 6_554 N
Sr2 O1 3.142(4) . 7_554 N
Sr2 O1 3.142(4) . 8_554 N
Sr2 O1 2.657(4) . -5_465 N
Sr2 O1 2.657(4) . -6_445 N
Sr2 O1 2.657(4) . -7_645 N
Sr2 O1 2.657(4) . -8_665 N
Sr2 O2 2.511(7) . 1_555 N
Sr2 O2 2.870(7) . 5_554 N
Si1 Sr1 3.2615(4) . 1_554 N
Si1 Sr1 3.2615(4) . 3_564 N
Si1 Sr1 3.2615(4) . 5_554 N
Si1 Sr1 3.2615(4) . 7_564 N
Si1 Sr2 3.47689(4) . 1_555 N
Si1 Sr2 3.47689(4) . 1_565 N
Si1 Sr2 3.47689(4) . -1_565 N
Si1 Sr2 3.47689(4) . -1_665 N
Si1 O1 1.6294(33) . 5_554 N
Si1 O1 1.6294(33) . 7_564 N
Si1 O1 1.6294(33) . -6_455 N
Si1 O1 1.6294(33) . -8_665 N
O1 Sr1 2.6642(34) . 1_555 N
O1 Sr1 2.4909(32) . 2_655 N
O1 Sr1 2.989(4) . 3_565 N
O1 Sr2 3.142(4) . 5_555 N
O1 Sr2 2.657(4) . -5_565 N
O1 Si1 1.6294(33) . 5_555 N
O2 Sr1 2.5477(8) . 5_544 N
O2 Sr1 2.5477(8) . 6_654 N
O2 Sr1 2.5477(8) . 7_564 N
O2 Sr1 2.5477(8) . 8_454 N
O2 Sr2 2.511(7) . 1_555 N
O2 Sr2 2.870(7) . 5_555 N
